At low temperatures around 300K, the yield strength either decreases or does not change with temperature. At moderate temperatures (0.35-0.45 T m), yield strength has been observed to increase with an increased vacancy concentration, providing further evidence for a vacancy driven strengthening mechanism. The increase in yield strength from increased vacancy concentration is believed to be the result of dislocations being pinned by vacancies on the slip plane, causing the dislocations to bow. Then, above the peak stress temperature, vacancies can migrate as vacancy migration is easier with elevated temperatures. At those temperatures, vacancies no longer hinder dislocation motion but rather aid climb. In the vacancy strengthening model, the increased strength below the peak stress temperature is approximated as proportional to the vacancy concentration to the one-half with the vacancy concentration estimated using Maxwell-Boltzmann statistics. Thus, the strength can be estimated as e − − E f / 2 k B T , with E f being the vacancy formation energy and T being the absolute temperature. Above the peak stress temperature, a diffusion-assisted deformation mechanism can be used to describe strength since vacancies are now mobile and assist dislocation motion. Above the peak, the yield strength is strain rate dependent and thus, the peak yield strength is rate dependent. As a result, the peak stress temperature increases with an increased strain rate. Note, this is different than the yield strength anomaly, which is the yield strength below the peak, being rate dependent. The peak yield strength is also dependent on percent aluminum in the FeAl alloy. As the percent aluminum increases, the peak yield strength occurs at lower temperatures.